#------------------------------------------------------------------------------
#$Date: 2023-03-20 11:26:05 +0200 (Mon, 20 Mar 2023) $
#$Revision: 281946 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/19/4001959.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001959
loop_
_publ_author_name
'Blankenship, Trevor V.'
'Chen, Banghao'
'Latturner, Susan E.'
_publ_section_title
;
 Ca54In13B4--xH23+x: A Complex Metal Subhydride Featuring Ionic and
 Metallic Regions
;
_journal_issue                   10
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3202
_journal_paper_doi               10.1021/cm5007982
_journal_volume                  26
_journal_year                    2014
_chemical_formula_sum            'B4 Ca53 H23 In13'
_chemical_formula_weight         3752.14
_space_group_IT_number           204
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   16.3608(6)
_cell_length_b                   16.3608(6)
_cell_length_c                   16.3608(6)
_cell_measurement_temperature    173(2)
_cell_volume                     4379.4(3)
_computing_cell_refinement       'Saint (Bruker, 2008)'
_computing_data_collection       'APEX2 (Bruker, 2008)'
_computing_data_reduction        'Saint (Bruker, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measurement_device_type  'Bruker APEX-II CCD area-detector'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0236
_diffrn_reflns_av_sigmaI/netI    0.0075
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            24720
_diffrn_reflns_theta_full        28.22
_diffrn_reflns_theta_max         28.22
_diffrn_reflns_theta_min         1.76
_exptl_absorpt_coefficient_mu    6.467
_exptl_absorpt_correction_T_max  0.879
_exptl_absorpt_correction_T_min  0.792
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2008)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    2.845
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       spheroid
_exptl_crystal_F_000             3526
_exptl_crystal_size_max          0.04
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.978
_refine_diff_density_min         -0.553
_refine_diff_density_rms         0.088
_refine_ls_extinction_coef       0.000020(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.142
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     62
_refine_ls_number_reflns         988
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.164
_refine_ls_R_factor_all          0.0171
_refine_ls_R_factor_gt           0.0165
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0138P)²+20.0180P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0395
_refine_ls_wR_factor_ref         0.0397
_reflns_number_gt                958
_reflns_number_total             988
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm5007982_si_002.cif
_cod_data_source_block           tb201dCaInBHe
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4001958--4001959.cif.
;
_cod_original_sg_symbol_H-M      Im-3
_cod_original_formula_sum        'B4 Ca53 He23 In13'
_cod_database_code               4001959
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
In1 In 0.0000 0.0000 0.0000 0.01132(15) Uani 1 24 d S
In2 In 0.0000 0.209286(14) 0.338031(14) 0.01563(9) Uani 1 2 d S
Ca1 Ca 0.0000 0.10896(4) 0.17264(4) 0.01612(14) Uani 1 2 d S
Ca2 Ca 0.0000 0.0000 0.35830(6) 0.01670(19) Uani 1 4 d S
Ca3 Ca 0.18401(3) 0.11348(3) 0.29807(3) 0.02317(13) Uani 1 1 d .
Ca4 Ca 0.0000 0.39805(12) 0.3819(2) 0.0388(9) Uani 0.568(6) 2 d SP
Ca5 Ca 0.0000 0.3222(3) 0.5000 0.0282(12) Uani 0.282(4) 4 d SP
Ca6 Ca 0.0000 0.4078(3) 0.3214(8) 0.041(3) Uani 0.181(6) 2 d SP
H1 H- 0.1471(7) 0.1471(7) 0.1471(7) 0.048(5) Uani 1 3 d S
H2 H- 0.0889(13) 0.0000 0.2353(13) 0.082(6) Uani 1 2 d S
B3 B 0.2500 0.2500 0.2500 0.024(4) Uani 0.41(6) 6 d SP
H3 H- 0.2500 0.2500 0.2500 0.024(4) Uani 0.59(6) 6 d SP
H4 H- 0.0000 0.0000 0.5000 0.014(4) Uani 1 8 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H- H- 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ca1 In1 Ca1 180.00(2) . 25
Ca1 In1 Ca1 116.831(5) . 33
Ca1 In1 Ca1 63.169(5) 25 33
Ca1 In1 Ca1 63.169(5) . 9
Ca1 In1 Ca1 116.831(5) 25 9
Ca1 In1 Ca1 180.00(2) 33 9
Ca1 In1 Ca1 116.831(5) . 29
Ca1 In1 Ca1 63.169(5) 25 29
Ca1 In1 Ca1 63.169(5) 33 29
Ca1 In1 Ca1 116.831(5) 9 29
Ca1 In1 Ca1 63.169(5) . 5
Ca1 In1 Ca1 116.831(5) 25 5
Ca1 In1 Ca1 116.831(5) 33 5
Ca1 In1 Ca1 63.169(5) 9 5
Ca1 In1 Ca1 180.00(2) 29 5
Ca1 In1 Ca1 116.831(5) . 34
Ca1 In1 Ca1 63.169(5) 25 34
Ca1 In1 Ca1 64.52(2) 33 34
Ca1 In1 Ca1 115.48(2) 9 34
Ca1 In1 Ca1 116.831(5) 29 34
Ca1 In1 Ca1 63.169(5) 5 34
Ca1 In1 Ca1 116.831(5) . 6
Ca1 In1 Ca1 63.169(5) 25 6
Ca1 In1 Ca1 116.831(5) 33 6
Ca1 In1 Ca1 63.169(5) 9 6
Ca1 In1 Ca1 115.48(2) 29 6
Ca1 In1 Ca1 64.52(2) 5 6
Ca1 In1 Ca1 63.169(5) 34 6
Ca1 In1 Ca1 63.169(5) . 30
Ca1 In1 Ca1 116.831(5) 25 30
Ca1 In1 Ca1 63.169(5) 33 30
Ca1 In1 Ca1 116.831(5) 9 30
Ca1 In1 Ca1 64.52(2) 29 30
Ca1 In1 Ca1 115.48(2) 5 30
Ca1 In1 Ca1 116.831(5) 34 30
Ca1 In1 Ca1 180.00(2) 6 30
Ca1 In1 Ca1 115.48(2) . 26
Ca1 In1 Ca1 64.52(2) 25 26
Ca1 In1 Ca1 116.831(5) 33 26
Ca1 In1 Ca1 63.169(5) 9 26
Ca1 In1 Ca1 63.169(5) 29 26
Ca1 In1 Ca1 116.831(5) 5 26
Ca1 In1 Ca1 116.831(5) 34 26
Ca1 In1 Ca1 63.169(5) 6 26
Ca1 In1 Ca1 116.831(5) 30 26
Ca1 In1 Ca1 64.52(2) . 2
Ca1 In1 Ca1 115.48(2) 25 2
Ca1 In1 Ca1 63.169(5) 33 2
Ca1 In1 Ca1 116.831(5) 9 2
Ca1 In1 Ca1 116.831(5) 29 2
Ca1 In1 Ca1 63.169(5) 5 2
Ca1 In1 Ca1 63.169(5) 34 2
Ca1 In1 Ca1 116.831(5) 6 2
Ca1 In1 Ca1 63.169(5) 30 2
Ca1 In1 Ca1 180.00(2) 26 2
Ca1 In1 Ca1 63.169(5) . 10
Ca1 In1 Ca1 116.831(5) 25 10
Ca1 In1 Ca1 115.48(2) 33 10
Ca1 In1 Ca1 64.52(2) 9 10
Ca1 In1 Ca1 63.169(5) 29 10
Ca1 In1 Ca1 116.831(5) 5 10
Ca1 In1 Ca1 180.00(2) 34 10
Ca1 In1 Ca1 116.831(5) 6 10
Ca1 In1 Ca1 63.169(5) 30 10
Ca1 In1 Ca1 63.169(5) 26 10
Ca1 In1 Ca1 116.831(5) 2 10
Ca6 In2 Ca6 58.45(16) 45 46_455
Ca6 In2 Ca1 130.5(2) 45 .
Ca6 In2 Ca1 130.5(2) 46_455 .
Ca6 In2 Ca4 87.95(19) 45 .
Ca6 In2 Ca4 87.95(19) 46_455 .
Ca1 In2 Ca4 134.32(7) . .
Ca6 In2 Ca5 52.4(2) 45 .
Ca6 In2 Ca5 52.4(2) 46_455 .
Ca1 In2 Ca5 176.36(7) . .
Ca4 In2 Ca5 42.04(9) . .
Ca6 In2 Ca6 103.50(4) 45 .
Ca6 In2 Ca6 103.50(4) 46_455 .
Ca1 In2 Ca6 116.5(2) . .
Ca4 In2 Ca6 17.87(17) . .
Ca5 In2 Ca6 59.9(2) . .
Ca6 In2 Ca2 75.9(2) 45 .
Ca6 In2 Ca2 75.9(2) 46_455 .
Ca1 In2 Ca2 64.29(2) . .
Ca4 In2 Ca2 161.39(7) . .
Ca5 In2 Ca2 119.34(7) . .
Ca6 In2 Ca2 179.3(2) . .
Ca6 In2 Ca3 163.2(2) 45 35
Ca6 In2 Ca3 115.59(11) 46_455 35
Ca1 In2 Ca3 66.042(14) . 35
Ca4 In2 Ca3 75.83(6) . 35
Ca5 In2 Ca3 111.00(5) . 35
Ca6 In2 Ca3 61.29(18) . 35
Ca2 In2 Ca3 119.300(17) . 35
Ca6 In2 Ca3 115.59(11) 45 9
Ca6 In2 Ca3 163.2(2) 46_455 9
Ca1 In2 Ca3 66.042(14) . 9
Ca4 In2 Ca3 75.83(6) . 9
Ca5 In2 Ca3 111.00(5) . 9
Ca6 In2 Ca3 61.29(18) . 9
Ca2 In2 Ca3 119.300(17) . 9
Ca3 In2 Ca3 65.100(18) 35 9
Ca6 In2 Ca3 120.91(16) 45 28
Ca6 In2 Ca3 70.32(13) 46_455 28
Ca1 In2 Ca3 66.615(11) . 28
Ca4 In2 Ca3 118.982(11) . 28
Ca5 In2 Ca3 114.49(2) . 28
Ca6 In2 Ca3 115.86(6) . 28
Ca2 In2 Ca3 64.333(10) . 28
Ca3 In2 Ca3 65.428(18) 35 28
Ca3 In2 Ca3 121.425(15) 9 28
Ca6 In2 Ca3 70.32(13) 45 .
Ca6 In2 Ca3 120.91(16) 46_455 .
Ca1 In2 Ca3 66.615(11) . .
Ca4 In2 Ca3 118.982(11) . .
Ca5 In2 Ca3 114.49(2) . .
Ca6 In2 Ca3 115.86(6) . .
Ca2 In2 Ca3 64.333(10) . .
Ca3 In2 Ca3 121.425(15) 35 .
Ca3 In2 Ca3 65.427(18) 9 .
Ca3 In2 Ca3 121.141(19) 28 .
Ca6 In2 Ca4 16.30(19) 45 45
Ca6 In2 Ca4 60.65(10) 46_455 45
Ca1 In2 Ca4 115.48(5) . 45
Ca4 In2 Ca4 104.241(13) . 45
Ca5 In2 Ca4 67.61(8) . 45
Ca6 In2 Ca4 119.49(15) . 45
Ca2 In2 Ca4 59.88(5) . 45
Ca3 In2 Ca4 176.16(3) 35 45
Ca3 In2 Ca4 118.70(3) 9 45
Ca3 In2 Ca4 111.61(3) 28 45
Ca3 In2 Ca4 62.01(4) . 45
H2 Ca1 H2 144.6(4) 9 2
H2 Ca1 H2 144.6(4) 9 .
H2 Ca1 H2 70.5(8) 2 .
H2 Ca1 H1 72.671(16) 9 .
H2 Ca1 H1 142.5(4) 2 .
H2 Ca1 H1 72.0(4) . .
H2 Ca1 H1 72.671(16) 9 28
H2 Ca1 H1 72.0(4) 2 28
H2 Ca1 H1 142.5(4) . 28
H1 Ca1 H1 145.34(3) . 28
H2 Ca1 In2 92.3(5) 9 .
H2 Ca1 In2 91.1(4) 2 .
H2 Ca1 In2 91.1(4) . .
H1 Ca1 In2 90.8(3) . .
H1 Ca1 In2 90.8(3) 28 .
H2 Ca1 In1 88.7(5) 9 .
H2 Ca1 In1 88.1(4) 2 .
H2 Ca1 In1 88.1(4) . .
H1 Ca1 In1 89.5(3) . .
H1 Ca1 In1 89.5(3) 28 .
In2 Ca1 In1 178.98(2) . .
H2 Ca1 Ca1 105.1(3) 9 30
H2 Ca1 Ca1 45.1(5) 2 30
H2 Ca1 Ca1 103.1(3) . 30
H1 Ca1 Ca1 147.9(3) . 30
H1 Ca1 Ca1 46.0(2) 28 30
In2 Ca1 Ca1 121.254(11) . 30
In1 Ca1 Ca1 58.416(3) . 30
H2 Ca1 Ca1 105.1(3) 9 5
H2 Ca1 Ca1 103.1(3) 2 5
H2 Ca1 Ca1 45.1(5) . 5
H1 Ca1 Ca1 46.0(2) . 5
H1 Ca1 Ca1 147.9(3) 28 5
In2 Ca1 Ca1 121.254(11) . 5
In1 Ca1 Ca1 58.416(3) . 5
Ca1 Ca1 Ca1 107.665(7) 30 5
H2 Ca1 Ca1 46.0(3) 9 10
H2 Ca1 Ca1 104.2(5) 2 10
H2 Ca1 Ca1 146.5(4) . 10
H1 Ca1 Ca1 106.18(19) . 10
H1 Ca1 Ca1 46.0(2) 28 10
In2 Ca1 Ca1 122.398(16) . 10
In1 Ca1 Ca1 58.416(3) . 10
Ca1 Ca1 Ca1 60.0 30 10
Ca1 Ca1 Ca1 108.826(17) 5 10
H2 Ca1 Ca1 46.0(3) 9 9
H2 Ca1 Ca1 146.5(4) 2 9
H2 Ca1 Ca1 104.2(5) . 9
H1 Ca1 Ca1 46.0(2) . 9
H1 Ca1 Ca1 106.18(19) 28 9
In2 Ca1 Ca1 122.398(16) . 9
In1 Ca1 Ca1 58.416(3) . 9
Ca1 Ca1 Ca1 108.826(17) 30 9
Ca1 Ca1 Ca1 60.0 5 9
Ca1 Ca1 Ca1 61.27(3) 10 9
H2 Ca1 Ca2 154.0(5) 9 .
H2 Ca1 Ca2 44.8(5) 2 .
H2 Ca1 Ca2 44.8(5) . .
H1 Ca1 Ca2 105.57(16) . .
H1 Ca1 Ca2 105.57(16) 28 .
In2 Ca1 Ca2 61.648(15) . .
In1 Ca1 Ca2 117.33(2) . .
Ca1 Ca1 Ca2 89.94(2) 30 .
Ca1 Ca1 Ca2 89.94(2) 5 .
Ca1 Ca1 Ca2 147.882(18) 10 .
Ca1 Ca1 Ca2 147.882(18) 9 .
H4 Ca2 H2 144.2(5) . 2
H4 Ca2 H2 144.2(5) . .
H2 Ca2 H2 71.7(10) 2 .
H4 Ca2 In2 95.531(17) . .
H2 Ca2 In2 85.52(3) 2 .
H2 Ca2 In2 85.52(3) . .
H4 Ca2 In2 95.532(17) . 2
H2 Ca2 In2 85.52(3) 2 2
H2 Ca2 In2 85.52(3) . 2
In2 Ca2 In2 168.94(3) . 2
H4 Ca2 Ca4 47.75(3) . 45
H2 Ca2 Ca4 145.92(6) 2 45
H2 Ca2 Ca4 105.2(4) . 45
In2 Ca2 Ca4 60.47(6) . 45
In2 Ca2 Ca4 128.50(6) 2 45
H4 Ca2 Ca4 47.75(3) . 46_455
H2 Ca2 Ca4 105.2(4) 2 46_455
H2 Ca2 Ca4 145.92(6) . 46_455
In2 Ca2 Ca4 60.47(6) . 46_455
In2 Ca2 Ca4 128.50(6) 2 46_455
Ca4 Ca2 Ca4 57.86(9) 45 46_455
H4 Ca2 Ca4 47.75(3) . 22_545
H2 Ca2 Ca4 145.92(6) 2 22_545
H2 Ca2 Ca4 105.2(4) . 22_545
In2 Ca2 Ca4 128.50(6) . 22_545
In2 Ca2 Ca4 60.47(6) 2 22_545
Ca4 Ca2 Ca4 68.16(11) 45 22_545
Ca4 Ca2 Ca4 95.51(6) 46_455 22_545
H4 Ca2 Ca4 47.75(3) . 21_445
H2 Ca2 Ca4 105.2(4) 2 21_445
H2 Ca2 Ca4 145.92(6) . 21_445
In2 Ca2 Ca4 128.50(6) . 21_445
In2 Ca2 Ca4 60.47(6) 2 21_445
Ca4 Ca2 Ca4 95.51(6) 45 21_445
Ca4 Ca2 Ca4 68.16(11) 46_455 21_445
Ca4 Ca2 Ca4 57.86(9) 22_545 21_445
H4 Ca2 Ca1 149.591(14) . 2
H2 Ca2 Ca1 45.6(3) 2 2
H2 Ca2 Ca1 45.6(3) . 2
In2 Ca2 Ca1 114.88(3) . 2
In2 Ca2 Ca1 54.060(14) 2 2
Ca4 Ca2 Ca1 149.71(3) 45 2
Ca4 Ca2 Ca1 149.71(3) 46_455 2
Ca4 Ca2 Ca1 107.23(4) 22_545 2
Ca4 Ca2 Ca1 107.23(4) 21_445 2
H4 Ca2 Ca1 149.592(14) . .
H2 Ca2 Ca1 45.6(3) 2 .
H2 Ca2 Ca1 45.6(3) . .
In2 Ca2 Ca1 54.061(14) . .
In2 Ca2 Ca1 114.88(3) 2 .
Ca4 Ca2 Ca1 107.23(4) 45 .
Ca4 Ca2 Ca1 107.23(4) 46_455 .
Ca4 Ca2 Ca1 149.71(3) 22_545 .
Ca4 Ca2 Ca1 149.71(3) 21_445 .
Ca1 Ca2 Ca1 60.82(3) 2 .
H4 Ca2 Ca3 105.567(18) . 2
H2 Ca2 Ca3 45.8(4) 2 2
H2 Ca2 Ca3 105.2(4) . 2
In2 Ca2 Ca3 118.519(13) . 2
In2 Ca2 Ca3 58.050(9) 2 2
Ca4 Ca2 Ca3 149.36(4) 45 2
Ca4 Ca2 Ca3 93.85(5) 46_455 2
Ca4 Ca2 Ca3 107.08(6) 22_545 2
Ca4 Ca2 Ca3 60.03(2) 21_445 2
Ca1 Ca2 Ca3 60.831(14) 2 2
Ca1 Ca2 Ca3 91.40(2) . 2
H1 Ca3 B3 68.2(3) . .
H1 Ca3 H2 69.0(5) . .
B3 Ca3 H2 137.1(4) . .
H1 Ca3 Ca6 139.88(12) . 5
B3 Ca3 Ca6 110.57(15) . 5
H2 Ca3 Ca6 102.1(3) . 5
H1 Ca3 In2 83.31(3) . 5
B3 Ca3 In2 91.811(14) . 5
H2 Ca3 In2 83.6(4) . 5
Ca6 Ca3 In2 56.59(12) 5 5
H1 Ca3 In2 83.20(3) . .
B3 Ca3 In2 91.679(15) . .
H2 Ca3 In2 83.0(4) . .
Ca6 Ca3 In2 135.94(14) 5 .
In2 Ca3 In2 163.67(2) 5 .
H1 Ca3 Ca4 141.95(9) . 45
B3 Ca3 Ca4 114.70(5) . 45
H2 Ca3 Ca4 98.9(5) . 45
Ca6 Ca3 Ca4 76.89(12) 5 45
In2 Ca3 Ca4 132.54(6) 5 45
In2 Ca3 Ca4 59.16(5) . 45
H1 Ca3 Ca1 44.2(3) . 5
B3 Ca3 Ca1 101.748(18) . 5
H2 Ca3 Ca1 43.3(5) . 5
Ca6 Ca3 Ca1 101.77(7) 5 5
In2 Ca3 Ca1 53.176(13) 5 5
In2 Ca3 Ca1 110.498(18) . 5
Ca4 Ca3 Ca1 141.69(4) 45 5
H1 Ca3 Ca3 101.8(3) . 45
B3 Ca3 Ca3 45.822(9) . 45
H2 Ca3 Ca3 148.6(4) . 45
Ca6 Ca3 Ca3 64.80(15) 5 45
In2 Ca3 Ca3 65.268(10) 5 45
In2 Ca3 Ca3 126.823(17) . 45
Ca4 Ca3 Ca3 105.10(3) 45 45
Ca1 Ca3 Ca3 108.738(17) 5 45
H1 Ca3 Ca3 101.8(3) . 41
B3 Ca3 Ca3 45.822(9) . 41
H2 Ca3 Ca3 148.0(4) . 41
Ca6 Ca3 Ca3 103.48(7) 5 41
In2 Ca3 Ca3 126.896(17) 5 41
In2 Ca3 Ca3 65.211(11) . 41
Ca4 Ca3 Ca3 68.99(5) 45 41
Ca1 Ca3 Ca3 144.603(14) 5 41
Ca3 Ca3 Ca3 61.94(2) 45 41
H1 Ca3 Ca1 43.8(2) . .
B3 Ca3 Ca1 100.951(19) . .
H2 Ca3 Ca1 43.7(3) . .
Ca6 Ca3 Ca1 145.76(11) 5 .
In2 Ca3 Ca1 110.813(18) 5 .
In2 Ca3 Ca1 52.858(12) . .
Ca4 Ca3 Ca1 102.19(3) 45 .
Ca1 Ca3 Ca1 57.64(2) 5 .
Ca3 Ca3 Ca1 143.920(16) 45 .
Ca3 Ca3 Ca1 108.057(17) 41 .
Ca6 Ca4 Ca5 156.4(4) . .
Ca6 Ca4 H4 130.1(4) . 17_455
Ca5 Ca4 H4 73.52(14) . 17_455
Ca6 Ca4 In2 86.0(3) . .
Ca5 Ca4 In2 70.36(11) . .
H4 Ca4 In2 143.89(14) 17_455 .
Ca6 Ca4 Ca6 63.6(3) . 2_565
Ca5 Ca4 Ca6 140.02(19) . 2_565
H4 Ca4 Ca6 66.5(2) 17_455 2_565
In2 Ca4 Ca6 149.62(14) . 2_565
Ca6 Ca4 Ca4 80.9(3) . 2_565
Ca5 Ca4 Ca4 122.72(10) . 2_565
H4 Ca4 Ca4 49.20(8) 17_455 2_565
In2 Ca4 Ca4 166.92(7) . 2_565
Ca6 Ca4 Ca4 17.30(18) 2_565 2_565
Ca6 Ca4 Ca2 118.5(2) . 41
Ca5 Ca4 Ca2 77.88(10) . 41
H4 Ca4 Ca2 42.25(3) 17_455 41
In2 Ca4 Ca2 126.73(7) . 41
Ca6 Ca4 Ca2 72.83(16) 2_565 41
Ca4 Ca4 Ca2 61.07(4) 2_565 41
Ca6 Ca4 Ca2 118.5(2) . 17_455
Ca5 Ca4 Ca2 77.88(10) . 17_455
H4 Ca4 Ca2 42.25(3) 17_455 17_455
In2 Ca4 Ca2 126.73(7) . 17_455
Ca6 Ca4 Ca2 72.83(16) 2_565 17_455
Ca4 Ca4 Ca2 61.07(4) 2_565 17_455
Ca2 Ca4 Ca2 84.49(6) 41 17_455
Ca6 Ca4 In2 59.94(18) . 41
Ca5 Ca4 In2 128.45(6) . 41
H4 Ca4 In2 90.65(4) 17_455 41
In2 Ca4 In2 111.78(5) . 41
Ca6 Ca4 In2 54.05(5) 2_565 41
Ca4 Ca4 In2 61.26(2) 2_565 41
Ca2 Ca4 In2 59.651(19) 41 41
Ca2 Ca4 In2 121.47(5) 17_455 41
Ca6 Ca4 In2 59.94(18) . 18_455
Ca5 Ca4 In2 128.45(6) . 18_455
H4 Ca4 In2 90.65(4) 17_455 18_455
In2 Ca4 In2 111.78(5) . 18_455
Ca6 Ca4 In2 54.05(5) 2_565 18_455
Ca4 Ca4 In2 61.26(2) 2_565 18_455
Ca2 Ca4 In2 121.47(5) 41 18_455
Ca2 Ca4 In2 59.651(19) 17_455 18_455
In2 Ca4 In2 99.64(9) 41 18_455
Ca6 Ca4 Ca3 94.62(12) . 18_455
Ca5 Ca4 Ca3 77.22(6) . 18_455
H4 Ca4 Ca3 103.29(6) 17_455 18_455
In2 Ca4 Ca3 68.79(3) . 18_455
Ca6 Ca4 Ca3 111.45(4) 2_565 18_455
Ca4 Ca4 Ca3 112.11(3) 2_565 18_455
Ca2 Ca4 Ca3 142.46(10) 41 18_455
Ca2 Ca4 Ca3 63.09(2) 17_455 18_455
In2 Ca4 Ca3 153.87(11) 41 18_455
In2 Ca4 Ca3 58.833(16) 18_455 18_455
Ca6 Ca4 Ca3 94.62(12) . 41
Ca5 Ca4 Ca3 77.22(6) . 41
H4 Ca4 Ca3 103.29(6) 17_455 41
In2 Ca4 Ca3 68.79(3) . 41
Ca6 Ca4 Ca3 111.45(4) 2_565 41
Ca4 Ca4 Ca3 112.11(3) 2_565 41
Ca2 Ca4 Ca3 63.09(2) 41 41
Ca2 Ca4 Ca3 142.46(10) 17_455 41
In2 Ca4 Ca3 58.833(16) 41 41
In2 Ca4 Ca3 153.87(11) 18_455 41
Ca3 Ca4 Ca3 135.71(7) 18_455 41
Ca4 Ca5 Ca4 114.6(2) . 26_556
Ca4 Ca5 Ca6 117.05(9) . 46_455
Ca4 Ca5 Ca6 117.05(9) 26_556 46_455
Ca4 Ca5 Ca6 117.05(9) . 45
Ca4 Ca5 Ca6 117.05(9) 26_556 45
Ca6 Ca5 Ca6 65.4(3) 46_455 45
Ca4 Ca5 H4 57.28(10) . 17_455
Ca4 Ca5 H4 57.28(10) 26_556 17_455
Ca6 Ca5 H4 147.29(16) 46_455 17_455
Ca6 Ca5 H4 147.29(16) 45 17_455
Ca4 Ca5 In2 67.59(5) . .
Ca4 Ca5 In2 177.84(17) 26_556 .
Ca6 Ca5 In2 61.24(9) 46_455 .
Ca6 Ca5 In2 61.24(9) 45 .
H4 Ca5 In2 124.88(7) 17_455 .
Ca4 Ca5 In2 177.84(17) . 26_556
Ca4 Ca5 In2 67.59(5) 26_556 26_556
Ca6 Ca5 In2 61.24(9) 46_455 26_556
Ca6 Ca5 In2 61.24(9) 45 26_556
H4 Ca5 In2 124.87(7) 17_455 26_556
In2 Ca5 In2 110.25(13) . 26_556
Ca4 Ca5 Ca6 7.11(12) . .
Ca4 Ca5 Ca6 121.7(2) 26_556 .
Ca6 Ca5 Ca6 111.32(14) 46_455 .
Ca6 Ca5 Ca6 111.32(14) 45 .
H4 Ca5 Ca6 64.39(14) 17_455 .
In2 Ca5 Ca6 60.48(12) . .
In2 Ca5 Ca6 170.73(18) 26_556 .
Ca4 Ca5 Ca6 121.7(2) . 26_556
Ca4 Ca5 Ca6 7.11(12) 26_556 26_556
Ca6 Ca5 Ca6 111.33(14) 46_455 26_556
Ca6 Ca5 Ca6 111.33(14) 45 26_556
H4 Ca5 Ca6 64.39(14) 17_455 26_556
In2 Ca5 Ca6 170.73(18) . 26_556
In2 Ca5 Ca6 60.48(12) 26_556 26_556
Ca6 Ca5 Ca6 128.8(3) . 26_556
Ca4 Ca5 Ca2 64.99(9) . 41
Ca4 Ca5 Ca2 64.99(9) 26_556 41
Ca6 Ca5 Ca2 174.16(18) 46_455 41
Ca6 Ca5 Ca2 108.74(16) 45 41
H4 Ca5 Ca2 38.55(4) 17_455 41
In2 Ca5 Ca2 116.56(3) . 41
In2 Ca5 Ca2 116.56(3) 26_556 41
Ca6 Ca5 Ca2 70.24(11) . 41
Ca6 Ca5 Ca2 70.24(11) 26_556 41
Ca4 Ca5 Ca2 64.99(9) . 17_455
Ca4 Ca5 Ca2 64.99(9) 26_556 17_455
Ca6 Ca5 Ca2 108.74(16) 46_455 17_455
Ca6 Ca5 Ca2 174.16(18) 45 17_455
H4 Ca5 Ca2 38.55(4) 17_455 17_455
In2 Ca5 Ca2 116.56(3) . 17_455
In2 Ca5 Ca2 116.56(3) 26_556 17_455
Ca6 Ca5 Ca2 70.24(11) . 17_455
Ca6 Ca5 Ca2 70.24(11) 26_556 17_455
Ca2 Ca5 Ca2 77.10(9) 41 17_455
Ca4 Ca5 Ca4 118.92(9) . 46_455
Ca4 Ca5 Ca4 118.92(9) 26_556 46_455
Ca6 Ca5 Ca4 6.17(16) 46_455 46_455
Ca6 Ca5 Ca4 59.26(18) 45 46_455
H4 Ca5 Ca4 153.45(4) 17_455 46_455
In2 Ca5 Ca4 59.24(7) . 46_455
In2 Ca5 Ca4 59.24(7) 26_556 46_455
Ca6 Ca5 Ca4 112.75(12) . 46_455
Ca6 Ca5 Ca4 112.75(12) 26_556 46_455
Ca2 Ca5 Ca4 168.00(8) 41 46_455
Ca2 Ca5 Ca4 114.90(3) 17_455 46_455
Ca4 Ca6 Ca5 156.4(5) . 41
Ca4 Ca6 Ca6 99.1(3) . 2_565
Ca5 Ca6 Ca6 57.29(16) 41 2_565
Ca4 Ca6 In2 103.8(3) . 41
Ca5 Ca6 In2 66.38(17) 41 41
Ca6 Ca6 In2 60.77(8) 2_565 41
Ca4 Ca6 In2 103.8(3) . 18_455
Ca5 Ca6 In2 66.38(17) 41 18_455
Ca6 Ca6 In2 60.77(8) 2_565 18_455
In2 Ca6 In2 118.1(2) 41 18_455
Ca4 Ca6 Ca5 16.5(2) . .
Ca5 Ca6 Ca5 172.9(3) 41 .
Ca6 Ca6 Ca5 115.61(14) 2_565 .
In2 Ca6 Ca5 111.0(3) 41 .
In2 Ca6 Ca5 111.0(3) 18_455 .
Ca4 Ca6 In2 76.1(3) . .
Ca5 Ca6 In2 127.5(4) 41 .
Ca6 Ca6 In2 175.2(2) 2_565 .
In2 Ca6 In2 120.01(8) 41 .
In2 Ca6 In2 120.01(8) 18_455 .
Ca5 Ca6 In2 59.61(17) . .
Ca4 Ca6 H4 36.4(3) . 17_455
Ca5 Ca6 H4 119.97(17) 41 17_455
Ca6 Ca6 H4 62.68(13) 2_565 17_455
In2 Ca6 H4 85.43(17) 41 17_455
In2 Ca6 H4 85.43(17) 18_455 17_455
Ca5 Ca6 H4 52.9(2) . 17_455
In2 Ca6 H4 112.5(3) . 17_455
Ca4 Ca6 Ca4 81.8(4) . 2_565
Ca5 Ca6 Ca4 74.58(13) 41 2_565
Ca6 Ca6 Ca4 17.30(18) 2_565 2_565
In2 Ca6 Ca4 65.30(9) 41 2_565
In2 Ca6 Ca4 65.30(9) 18_455 2_565
Ca5 Ca6 Ca4 98.3(3) . 2_565
In2 Ca6 Ca4 157.9(4) . 2_565
H4 Ca6 Ca4 45.39(9) 17_455 2_565
Ca4 Ca6 Ca3 124.4(3) . 35
Ca5 Ca6 Ca3 74.4(3) 41 35
Ca6 Ca6 Ca3 121.61(11) 2_565 35
In2 Ca6 Ca3 127.9(4) 41 35
In2 Ca6 Ca3 71.59(14) 18_455 35
Ca5 Ca6 Ca3 111.44(15) . 35
In2 Ca6 Ca3 62.12(11) . 35
H4 Ca6 Ca3 145.48(16) 17_455 35
Ca4 Ca6 Ca3 134.08(19) 2_565 35
Ca4 Ca6 Ca3 124.4(3) . 9
Ca5 Ca6 Ca3 74.4(3) 41 9
Ca6 Ca6 Ca3 121.61(11) 2_565 9
In2 Ca6 Ca3 71.59(14) 41 9
In2 Ca6 Ca3 127.9(4) 18_455 9
Ca5 Ca6 Ca3 111.44(15) . 9
In2 Ca6 Ca3 62.12(11) . 9
H4 Ca6 Ca3 145.48(16) 17_455 9
Ca4 Ca6 Ca3 134.08(19) 2_565 9
Ca3 Ca6 Ca3 65.68(18) 35 9
Ca4 Ca6 Ca3 70.06(18) . 18_455
Ca5 Ca6 Ca3 116.84(18) 41 18_455
Ca6 Ca6 Ca3 113.39(7) 2_565 18_455
In2 Ca6 Ca3 171.3(3) 41 18_455
In2 Ca6 Ca3 59.38(3) 18_455 18_455
Ca5 Ca6 Ca3 64.81(15) . 18_455
In2 Ca6 Ca3 65.22(9) . 18_455
H4 Ca6 Ca3 86.1(2) 17_455 18_455
Ca4 Ca6 Ca3 107.18(15) 2_565 18_455
Ca3 Ca6 Ca3 60.21(5) 35 18_455
Ca3 Ca6 Ca3 116.78(16) 9 18_455
Ca1 H1 Ca1 87.9(5) 5 9
Ca1 H1 Ca1 87.9(5) 5 .
Ca1 H1 Ca1 87.9(5) 9 .
Ca1 H1 Ca3 89.70(2) 5 .
Ca1 H1 Ca3 177.3(7) 9 .
Ca1 H1 Ca3 90.68(2) . .
Ca1 H1 Ca3 177.3(7) 5 9
Ca1 H1 Ca3 90.68(2) 9 9
Ca1 H1 Ca3 89.70(2) . 9
Ca3 H1 Ca3 91.7(5) . 9
Ca1 H1 Ca3 90.68(2) 5 5
Ca1 H1 Ca3 89.70(2) 9 5
Ca1 H1 Ca3 177.3(7) . 5
Ca3 H1 Ca3 91.7(5) . 5
Ca3 H1 Ca3 91.7(5) 9 5
Ca1 H1 H2 53.0(4) 5 .
Ca1 H1 H2 121.4(8) 9 .
Ca1 H1 H2 54.0(4) . .
Ca3 H1 H2 56.0(4) . .
Ca3 H1 H2 126.2(4) 9 .
Ca3 H1 H2 126.6(4) 5 .
Ca1 H1 H2 121.4(8) 5 9
Ca1 H1 H2 54.0(4) 9 9
Ca1 H1 H2 53.0(4) . 9
Ca3 H1 H2 126.6(4) . 9
Ca3 H1 H2 56.0(4) 9 9
Ca3 H1 H2 126.2(4) 5 9
H2 H1 H2 106.9(6) . 9
Ca1 H1 H2 54.0(4) 5 5
Ca1 H1 H2 53.0(4) 9 5
Ca1 H1 H2 121.4(8) . 5
Ca3 H1 H2 126.2(4) . 5
Ca3 H1 H2 126.6(4) 9 5
Ca3 H1 H2 56.0(4) 5 5
H2 H1 H2 106.9(6) . 5
H2 H1 H2 106.9(6) 9 5
Ca1 H2 Ca2 177.7(10) 5 .
Ca1 H2 Ca1 88.8(6) 5 .
Ca2 H2 Ca1 89.5(6) . .
Ca1 H2 Ca1 88.8(6) 5 2
Ca2 H2 Ca1 89.5(6) . 2
Ca1 H2 Ca1 90.1(7) . 2
Ca1 H2 Ca3 89.9(6) 5 .
Ca2 H2 Ca3 91.7(6) . .
Ca1 H2 Ca3 90.05(3) . .
Ca1 H2 Ca3 178.7(9) 2 .
Ca1 H2 Ca3 89.9(6) 5 27
Ca2 H2 Ca3 91.7(6) . 27
Ca1 H2 Ca3 178.7(9) . 27
Ca1 H2 Ca3 90.05(3) 2 27
Ca3 H2 Ca3 89.7(7) . 27
Ca1 H2 H2 123.6(5) 5 2
Ca2 H2 H2 54.2(5) . 2
Ca1 H2 H2 54.7(4) . 2
Ca1 H2 H2 54.7(4) 2 2
Ca3 H2 H2 126.3(4) . 2
Ca3 H2 H2 126.3(4) 27 2
Ca1 H2 H1 54.3(4) 5 .
Ca2 H2 H1 125.7(4) . .
Ca1 H2 H1 54.0(3) . .
Ca1 H2 H1 124.2(9) 2 .
Ca3 H2 H1 55.1(4) . .
Ca3 H2 H1 125.0(8) 27 .
H2 H2 H1 108.7(4) 2 .
Ca1 H2 H1 54.3(4) 5 27
Ca2 H2 H1 125.7(4) . 27
Ca1 H2 H1 124.2(9) . 27
Ca1 H2 H1 54.0(3) 2 27
Ca3 H2 H1 125.0(8) . 27
Ca3 H2 H1 55.1(4) 27 27
H2 H2 H1 108.7(4) 2 27
H1 H2 H1 108.6(7) . 27
Ca3 B3 Ca3 88.357(17) . 45
Ca3 B3 Ca3 180.0 . 37
Ca3 B3 Ca3 91.644(17) 45 37
Ca3 B3 Ca3 91.643(17) . 5
Ca3 B3 Ca3 88.356(17) 45 5
Ca3 B3 Ca3 88.356(17) 37 5
Ca3 B3 Ca3 88.357(17) . 41
Ca3 B3 Ca3 91.644(17) 45 41
Ca3 B3 Ca3 91.644(17) 37 41
Ca3 B3 Ca3 180.000(12) 5 41
Ca3 B3 Ca3 91.643(17) . 9
Ca3 B3 Ca3 180.0 45 9
Ca3 B3 Ca3 88.356(17) 37 9
Ca3 B3 Ca3 91.644(17) 5 9
Ca3 B3 Ca3 88.356(17) 41 9
Ca2 H4 Ca2 180.0 25_556 .
Ca2 H4 Ca4 90.0 25_556 45
Ca2 H4 Ca4 90.0 . 45
Ca2 H4 Ca4 90.0 25_556 21_445
Ca2 H4 Ca4 90.0 . 21_445
Ca4 H4 Ca4 180.00(9) 45 21_445
Ca2 H4 Ca4 90.0 25_556 46_455
Ca2 H4 Ca4 90.0 . 46_455
Ca4 H4 Ca4 81.60(15) 45 46_455
Ca4 H4 Ca4 98.40(15) 21_445 46_455
Ca2 H4 Ca4 90.0 25_556 22_545
Ca2 H4 Ca4 90.0 . 22_545
Ca4 H4 Ca4 98.40(15) 45 22_545
Ca4 H4 Ca4 81.60(15) 21_445 22_545
Ca4 H4 Ca4 180.0 46_455 22_545
Ca2 H4 Ca5 90.0 25_556 45
Ca2 H4 Ca5 90.0 . 45
Ca4 H4 Ca5 49.20(8) 45 45
Ca4 H4 Ca5 130.80(8) 21_445 45
Ca4 H4 Ca5 130.80(8) 46_455 45
Ca4 H4 Ca5 49.20(8) 22_545 45
Ca2 H4 Ca5 90.0 25_556 21_445
Ca2 H4 Ca5 90.0 . 21_445
Ca4 H4 Ca5 130.80(8) 45 21_445
Ca4 H4 Ca5 49.20(8) 21_445 21_445
Ca4 H4 Ca5 49.20(8) 46_455 21_445
Ca4 H4 Ca5 130.80(8) 22_545 21_445
Ca5 H4 Ca5 180.0 45 21_445
Ca2 H4 Ca6 90.000(1) 25_556 45
Ca2 H4 Ca6 90.000(1) . 45
Ca4 H4 Ca6 13.49(11) 45 45
Ca4 H4 Ca6 166.51(11) 21_445 45
Ca4 H4 Ca6 68.12(19) 46_455 45
Ca4 H4 Ca6 111.88(19) 22_545 45
Ca5 H4 Ca6 62.68(13) 45 45
Ca5 H4 Ca6 117.32(13) 21_445 45
Ca2 H4 Ca6 90.000(1) 25_556 21_445
Ca2 H4 Ca6 90.000(1) . 21_445
Ca4 H4 Ca6 166.51(11) 45 21_445
Ca4 H4 Ca6 13.49(11) 21_445 21_445
Ca4 H4 Ca6 111.88(19) 46_455 21_445
Ca4 H4 Ca6 68.12(19) 22_545 21_445
Ca5 H4 Ca6 117.32(13) 45 21_445
Ca5 H4 Ca6 62.68(13) 21_445 21_445
Ca6 H4 Ca6 180.0 45 21_445
Ca2 H4 Ca6 90.0 25_556 46_455
Ca2 H4 Ca6 90.0 . 46_455
Ca4 H4 Ca6 68.12(18) 45 46_455
Ca4 H4 Ca6 111.88(19) 21_445 46_455
Ca4 H4 Ca6 13.49(11) 46_455 46_455
Ca4 H4 Ca6 166.51(11) 22_545 46_455
Ca5 H4 Ca6 117.32(13) 45 46_455
Ca5 H4 Ca6 62.68(13) 21_445 46_455
Ca6 H4 Ca6 54.6(3) 45 46_455
Ca6 H4 Ca6 125.4(3) 21_445 46_455
Ca2 H4 Ca6 90.0 25_556 22_545
Ca2 H4 Ca6 90.0 . 22_545
Ca4 H4 Ca6 111.88(19) 45 22_545
Ca4 H4 Ca6 68.12(19) 21_445 22_545
Ca4 H4 Ca6 166.51(11) 46_455 22_545
Ca4 H4 Ca6 13.49(11) 22_545 22_545
Ca5 H4 Ca6 62.68(13) 45 22_545
Ca5 H4 Ca6 117.32(13) 21_445 22_545
Ca6 H4 Ca6 125.4(3) 45 22_545
Ca6 H4 Ca6 54.6(3) 21_445 22_545
Ca6 H4 Ca6 180.000(1) 46_455 22_545
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
In1 Ca1 3.3400(7) .
In1 Ca1 3.3400(7) 25
In1 Ca1 3.3400(7) 33
In1 Ca1 3.3400(7) 9
In1 Ca1 3.3400(7) 29
In1 Ca1 3.3400(7) 5
In1 Ca1 3.3400(7) 34
In1 Ca1 3.3400(7) 6
In1 Ca1 3.3400(7) 30
In1 Ca1 3.3400(7) 26
In1 Ca1 3.3400(7) 2
In1 Ca1 3.3400(7) 10
In2 Ca6 3.091(3) 45
In2 Ca6 3.091(3) 46_455
In2 Ca1 3.1649(7) .
In2 Ca4 3.1706(17) .
In2 Ca5 3.230(3) .
In2 Ca6 3.259(5) .
In2 Ca2 3.4401(3) .
In2 Ca3 3.4507(5) 35
In2 Ca3 3.4507(5) 9
In2 Ca3 3.4565(5) 28
In2 Ca3 3.4565(5) .
In2 Ca4 3.468(2) 45
Ca1 H2 2.48(2) 9
Ca1 H2 2.518(15) 2
Ca1 H2 2.518(15) .
Ca1 H1 2.520(11) .
Ca1 H1 2.520(11) 28
Ca1 Ca1 3.4987(8) 30
Ca1 Ca1 3.4987(8) 5
Ca1 Ca1 3.4987(8) 10
Ca1 Ca1 3.4987(8) 9
Ca1 Ca2 3.5221(11) .
Ca2 H4 2.3184(10) .
Ca2 H2 2.48(2) 2
Ca2 H2 2.48(2) .
Ca2 In2 3.4402(3) 2
Ca2 Ca4 3.4483(19) 45
Ca2 Ca4 3.4483(19) 46_455
Ca2 Ca4 3.4483(19) 22_545
Ca2 Ca4 3.4483(19) 21_445
Ca2 Ca1 3.5220(11) 2
Ca2 Ca3 3.6716(6) 2
Ca3 H1 2.602(11) .
Ca3 B3 2.6025(5) .
Ca3 H2 2.632(15) .
Ca3 Ca6 3.424(8) 5
Ca3 In2 3.4506(5) 5
Ca3 Ca4 3.5669(10) 45
Ca3 Ca1 3.6130(8) 5
Ca3 Ca3 3.6274(9) 45
Ca3 Ca3 3.6274(9) 41
Ca4 Ca6 1.002(10) .
Ca4 Ca5 2.297(4) .
Ca4 H4 2.553(2) 17_455
Ca4 Ca6 3.328(5) 2_565
Ca4 Ca4 3.336(4) 2_565
Ca4 Ca2 3.4483(19) 41
Ca4 Ca2 3.4483(19) 17_455
Ca4 In2 3.469(2) 41
Ca4 In2 3.469(2) 18_455
Ca4 Ca3 3.5668(10) 18_455
Ca4 Ca3 3.5668(10) 41
Ca5 Ca4 2.297(4) 26_556
Ca5 Ca6 2.792(12) 46_455
Ca5 Ca6 2.792(12) 45
Ca5 H4 2.909(5) 17_455
Ca5 In2 3.230(3) 26_556
Ca5 Ca6 3.240(12) .
Ca5 Ca6 3.240(12) 26_556
Ca5 Ca2 3.720(4) 41
Ca5 Ca2 3.720(4) 17_455
Ca5 Ca4 3.732(6) 46_455
Ca6 Ca5 2.792(12) 41
Ca6 Ca6 3.018(10) 2_565
Ca6 In2 3.091(3) 41
Ca6 In2 3.091(3) 18_455
Ca6 H4 3.288(11) 17_455
Ca6 Ca4 3.328(5) 2_565
Ca6 Ca3 3.424(8) 35
Ca6 Ca3 3.424(8) 9
Ca6 Ca3 3.782(4) 18_455
H1 Ca1 2.520(11) 5
H1 Ca1 2.520(11) 9
H1 Ca3 2.602(11) 9
H1 Ca3 2.602(11) 5
H1 H2 2.963(14) .
H1 H2 2.963(14) 9
H1 H2 2.963(14) 5
H2 Ca1 2.48(2) 5
H2 Ca1 2.518(15) 2
H2 Ca3 2.632(15) 27
H2 H2 2.91(4) 2
H2 H1 2.963(14) 27
B3 Ca3 2.6026(5) 45
B3 Ca3 2.6026(5) 37
B3 Ca3 2.6026(5) 5
B3 Ca3 2.6026(5) 41
B3 Ca3 2.6026(5) 9
H4 Ca2 2.3183(10) 25_556
H4 Ca4 2.553(2) 45
H4 Ca4 2.553(2) 21_445
H4 Ca4 2.553(2) 46_455
H4 Ca4 2.553(2) 22_545
H4 Ca5 2.909(5) 45
H4 Ca5 2.909(5) 21_445
H4 Ca6 3.288(11) 45
H4 Ca6 3.288(11) 21_445
H4 Ca6 3.288(11) 46_455
H4 Ca6 3.288(11) 22_545
loop_
_cod_changelog_entry_id
_cod_changelog_entry_author
_cod_changelog_entry_date
_cod_changelog_entry_text
1 'Vaitkus, Antanas' 2023-03-20T11:25:00+02:00
;
 Updated the summary chemical formula and the atom site type symbols to
 represent hydride anions as 'H-' instead of 'He'. This allows to correctly
 recognise them as hydrogen atoms instead of helium atoms.
;
